金属学报  2020, Vol. 56 Issue (4): 558-582    DOI: 10.11900/0412.1961.2020.00058
 综述 本期目录 | 过刊浏览 |

1.上海大学材料科学与工程学院 上海 200444
2.钢铁研究总院 北京 100081
High Performance Steels: the Scenario of Theoryand Technology
DONG Han1,2(),LIAN Xintong1,HU Chundong1,LU Hengchang1,PENG Wei1,ZHAO Hongshan1,XU Dexiang1
1.School of Materials Science and Engineering, Shanghai University, Shanghai 200444, China
2.Central Iron and Steel Research Institute, Beijing 100081, China
 全文: PDF(33453 KB)   HTML

Abstract

Strengthening and toughening are the main topics of steels, and accompanied fatigue failure and delayed fracture requiring to be solved simultaneously. Not just more than that, better performances in fabrication and service are quite important for an intentional steel to be used eventually. It is worth to pay close attention to match up three main courses: steel processing, component fabrication and service evaluation. Over past two decades, ferrite grains can be refined to micron scale in both plain low carbon steel products and microalloyed steel products and lead to remarkable increase of strength. The reason to define the limitation of ferrite grain refinement to microns is ductility decrease, low processing efficiency and heat affected zone (HAZ) coarsening. Ten years ago, a novel microstructure M3 (multiphase, metastable and multiscale) was proposed to overcome the problems stated above, and led to ductility and/or toughness improvement. It based on the idea of crack initiation and propagation retardment. It led to prevalence of the 3rd generation advanced high strength steel (AHSS) and the 3rd generation high strength low alloy (HSLA) steel, presenting higher ductility and/or toughness at high strength level. In the near future, it is imaginable that polymorphic alloying will be taken into consideration instead of recent hot issue on microstructure control during whole processing. From the view point of classic alloying theory, solution and precipitation of alloying elements play an important role on processing and then final microstructure. The distribution and occurrence of small atom radius elements (e.g. C and N) and comparable atom radius elements (e.g. Cr, Mn, Ni, Co) in iron seem quite clear. The ambiguous situation still remains for B and P, and even larger atom radius elements such as rare earth (RE) elements. Segregation of small amount of them to defects and boundaries maybe lead to decrease of energy and result in remarkable change of microstructure characterization. Thanks to the advancement in processing and instrumentation technologies, the distribution and occurrence of alloying elements in steel and the advantages of different alloying elements in steel matrix and surface can be taken, so called the polymorphic alloying. The practices of polymorphic alloying in steel development are engaged to improve corrosion resistance, strengthening and toughening. The performance enhancements are discussed in cases of weathering steel microalloyed with RE, ultrahigh strength steel strengthening by carbide and intermetallic precipitates, bolt steel with C and microalloying elements, austenitic stainless steel alloyed with N, and martensitic stainless steel alloyed with C and Ag.

Key wordssteel    high performance    theory    technology

 ZTFLH: TG142

Corresponding author: Han DONG     E-mail: 13910077790@163.com

 服务 把本文推荐给朋友 加入引用管理器 E-mail Alert RSS 作者相关文章 董瀚 廉心桐 胡春东 陆恒昌 彭伟 赵洪山 徐德祥 44.8K

引用本文:

Han DONG, Xintong LIAN, Chundong HU, Hengchang LU, Wei PENG, Hongshan ZHAO, Dexiang XU. High Performance Steels: the Scenario of Theoryand Technology. Acta Metall Sin, 2020, 56(4): 558-582.

链接本文:

 表1  20世纪耐候钢的发展历程 图1  耐候钢锈层转变示意图 图2  稀土元素在钢中赋存示意图 图3  添加稀土前后的Q235和09CuPCrNi钢周期浸润腐蚀144 h后的样品形貌及腐蚀速率 图4  09CuPCrNiRE钢中Ce元素的AES谱 图5  钢铁材料强度的发展 图6  合金结构钢强度和塑韧性[17,18,19,20,21,22,23,24,25,26,27,28,29,30,31,32,33,34,35] 表2  钢铁材料常见韧化机制[42,43] 图7  0.15C5Mn3Al钢中裂纹在马氏体和铁素体中扩展[45] 图8  耐延迟断裂性能和抗疲劳性能随强度的提高而降低 图9  30Cr3Mo2V和25Cr2MoV钢中的碳化物形貌 表3  钢中不同氢陷阱的结合能(Ea)[51,54] 图10  A286样品显微组织及A286样品与进口产品在650 ℃持久实验后的性能对比 表4  航空航天用耐热紧固件用典型材料 表5  我国与日本非调质钢主要成分对比 (mass fraction / %) 图11  关键紧固件强度统计分布情况 图12  ZT35K-M钢在线退火组织 图13  一些氮合金化奥氏体不锈钢固溶后的室温力学性能[64,65,66,67,68,69,70] 图14  冷轧和固溶处理05Cr21Mn16Ni2N钢的工程应力-应变曲线 图15  奥氏体不锈钢耐点蚀当量(PREN)随N含量的变化 图16  不同N含量高氮奥氏体不锈钢和钛合金细胞毒性检验结果 表6  人群对Ni过敏的比例统计 表7  航发轴承钢的技术创新[89] 图17  6Cr16MoNiV钢和6Cr16MoVAgRE[93]钢夹杂物EDS 图18  不同高碳马氏体不锈钢的点蚀阻抗谱和腐蚀速率。 图19  6Cr16MoVAgRE钢EPMA分析 图20  6Cr16MoMA马氏体不锈钢SEM像和不同高碳马氏体不锈钢不同奥氏体化温度处理后试样冲击功